#------------------------------------------------------------------------------
#$Date: 2023-04-10 18:44:46 +0300 (Mon, 10 Apr 2023) $
#$Revision: 282534 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/01/67/2016784.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2016784
loop_
_publ_author_name
'Dordević, Tamara'
'Šutović, Sabina'
'Stojanović, Jovica'
'Karanović, Ljiljana'
_publ_section_title
;
 Sr, Ba and Cd arsenates with the apatite-type structure
;
_journal_coeditor_code           SQ3149
_journal_issue                   9
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              i82
_journal_page_last               i86
_journal_paper_doi               10.1107/S0108270108023457
_journal_volume                  64
_journal_year                    2008
_chemical_formula_iupac          'Cd5 (As O4)3 Cl10.58 (OH)0.42'
_chemical_formula_moiety         'As6 Cd10 Cl1.16 H0.84 O24.84'
_chemical_formula_structural     'Cd5 (AsO4)3 [Cl10.58 , (OH)0.42]'
_chemical_formula_sum            'As6 Cd10 Cl1.16 H0.84 O24.84'
_chemical_formula_weight         2012.93
_chemical_name_common            'Cadmium Chlorarsenate'
_chemical_name_systematic
;
cadmium arsenate hydroxide chloride
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   9.9710(10)
_cell_length_b                   9.9710(10)
_cell_length_c                   6.5140(10)
_cell_measurement_reflns_used    1387
_cell_measurement_temperature    294(2)
_cell_measurement_theta_max      30.034
_cell_measurement_theta_min      1.018
_cell_volume                     560.86(12)
_computing_cell_refinement       'SCALEPACK (Otwinowski & Minor, 1997)'
_computing_data_collection       'COLLECT (Nonius, 2002)'
_computing_data_reduction        'DENZO-SMN (Otwinowski & Minor, 1997)'
_computing_molecular_graphics    'ATOMS (Dowty, 2000)'
_computing_publication_material  'publCIF (Westrip, 2008)'
_computing_structure_refinement
;
WinGX (Farrugia, 1999) and SHELXL97 (Sheldrick, 2008)
;
_computing_structure_solution    'SIR97 (Altomare et al., 1999)'
_diffrn_ambient_temperature      294(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Nonius KappaCCD'
_diffrn_measurement_method       'φ and ω'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed X-ray tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0254
_diffrn_reflns_av_sigmaI/netI    0.0102
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            4589
_diffrn_reflns_theta_full        26.45
_diffrn_reflns_theta_max         26.45
_diffrn_reflns_theta_min         3.92
_exptl_absorpt_coefficient_mu    18.314
_exptl_absorpt_correction_T_max  0.396
_exptl_absorpt_correction_T_min  0.348
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
(Software?; Otwinowski & Minor, 1997; Otwinowski et al.,
2003)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    5.960
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             897.3
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.030
_refine_diff_density_min         -1.047
_refine_ls_extinction_coef       0.00154(16)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL97 (Sheldrick, 2008)'
_refine_ls_goodness_of_fit_ref   1.298
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     42
_refine_ls_number_reflns         424
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.296
_refine_ls_R_factor_all          0.0179
_refine_ls_R_factor_gt           0.0176
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+4.519P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0369
_refine_ls_wR_factor_ref         0.0370
_reflns_number_gt                420
_reflns_number_total             424
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            sq3149.cif
_cod_data_source_block           III
_cod_database_code               2016784
_cod_database_fobs_code          2016784
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-y, x-y, z'
'-x+y, -x, z'
'x-y, x, z+1/2'
'y, -x+y, z+1/2'
'-x, -y, -z'
'x, y, -z-1/2'
'y, -x+y, -z'
'x-y, x, -z'
'-x+y, -x, -z-1/2'
'-y, x-y, -z-1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
Cd Cd1 0.3333 0.6667 0.00216(8) 0.01110(17) Uani d S 1
Cd Cd2 0.26495(6) 0.02676(6) 0.2500 0.01741(17) Uani d S 1
As As1 0.40361(7) 0.37911(7) 0.2500 0.00749(17) Uani d S 1
Cl Cl1 0.0000 0.0000 0.2500 0.0247(19) Uani d SP 0.58(3)
O O4 0.0000 0.0000 0.2500 0.0247(19) Uani d SPD 0.42(3)
H H4 0.0000 0.0000 0.113(3) 0.030 Uiso d SPD 0.210(15)
O O1 0.3511(6) 0.5125(5) 0.2500 0.0125(9) Uani d S 1
O O2 0.6004(5) 0.4623(5) 0.2500 0.0126(10) Uani d S 1
O O3 0.3412(4) 0.2579(4) 0.0471(5) 0.0151(7) Uani d . 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O1 Cd1 O1 3_665 4_565 76.02(12)
O1 Cd1 O1 3_665 . 76.02(12)
O1 Cd1 O1 4_565 . 76.02(12)
O1 Cd1 O2 3_665 10 147.55(15)
O1 Cd1 O2 4_565 10 89.34(11)
O1 Cd1 O2 . 10 128.82(15)
O1 Cd1 O2 3_665 9_565 89.34(11)
O1 Cd1 O2 4_565 9_565 128.82(15)
O1 Cd1 O2 . 9_565 147.55(15)
O2 Cd1 O2 10 9_565 77.43(12)
O1 Cd1 O2 3_665 7_665 128.82(15)
O1 Cd1 O2 4_565 7_665 147.55(15)
O1 Cd1 O2 . 7_665 89.34(11)
O2 Cd1 O2 10 7_665 77.43(12)
O2 Cd1 O2 9_565 7_665 77.43(12)
O1 Cd1 O3 3_665 9_565 78.73(13)
O1 Cd1 O3 4_565 9_565 69.33(12)
O1 Cd1 O3 . 9_565 141.01(10)
O2 Cd1 O3 10 9_565 68.98(12)
O2 Cd1 O3 9_565 9_565 59.71(12)
O2 Cd1 O3 7_665 9_565 129.64(10)
O1 Cd1 O3 3_665 10 141.01(10)
O1 Cd1 O3 4_565 10 78.73(13)
O1 Cd1 O3 . 10 69.33(12)
O2 Cd1 O3 10 10 59.71(12)
O2 Cd1 O3 9_565 10 129.64(10)
O2 Cd1 O3 7_665 10 68.98(12)
O3 Cd1 O3 9_565 10 118.84(2)
O1 Cd1 O3 3_665 7_665 69.33(12)
O1 Cd1 O3 4_565 7_665 141.01(10)
O1 Cd1 O3 . 7_665 78.73(13)
O2 Cd1 O3 10 7_665 129.64(10)
O2 Cd1 O3 9_565 7_665 68.98(12)
O2 Cd1 O3 7_665 7_665 59.71(12)
O3 Cd1 O3 9_565 7_665 118.84(2)
O3 Cd1 O3 10 7_665 118.84(2)
O1 Cd1 Cd1 3_665 8_556 45.32(8)
O1 Cd1 Cd1 4_565 8_556 45.32(8)
O1 Cd1 Cd1 . 8_556 45.32(8)
O2 Cd1 Cd1 10 8_556 133.77(8)
O2 Cd1 Cd1 9_565 8_556 133.77(8)
O2 Cd1 Cd1 7_665 8_556 133.77(8)
O3 Cd1 Cd1 9_565 8_556 96.23(6)
O3 Cd1 Cd1 10 8_556 96.23(6)
O3 Cd1 Cd1 7_665 8_556 96.23(6)
O1 Cd1 Cd1 3_665 8 134.68(8)
O1 Cd1 Cd1 4_565 8 134.68(8)
O1 Cd1 Cd1 . 8 134.68(8)
O2 Cd1 Cd1 10 8 46.23(8)
O2 Cd1 Cd1 9_565 8 46.23(8)
O2 Cd1 Cd1 7_665 8 46.23(8)
O3 Cd1 Cd1 9_565 8 83.77(6)
O3 Cd1 Cd1 10 8 83.77(6)
O3 Cd1 Cd1 7_665 8 83.77(6)
Cd1 Cd1 Cd1 8_556 8 180.0
O1 Cd1 O3 3_665 4_565 104.83(12)
O1 Cd1 O3 4_565 4_565 40.80(9)
O1 Cd1 O3 . 4_565 110.56(12)
O2 Cd1 O3 10 4_565 50.67(9)
O2 Cd1 O3 9_565 4_565 101.07(11)
O2 Cd1 O3 7_665 4_565 126.10(11)
O3 Cd1 O3 9_565 4_565 49.18(9)
O3 Cd1 O3 10 4_565 72.46(9)
O3 Cd1 O3 7_665 4_565 168.01(8)
Cd1 Cd1 O3 8_556 4_565 85.93(5)
Cd1 Cd1 O3 8 4_565 94.07(5)
O3 Cd2 O3 9 6 122.43(18)
O3 Cd2 O2 9 3_655 88.65(10)
O3 Cd2 O2 6 3_655 88.65(10)
O3 Cd2 O3 9 8_556 150.03(14)
O3 Cd2 O3 6 8_556 84.92(6)
O2 Cd2 O3 3_655 8_556 79.28(12)
O3 Cd2 O3 9 . 84.92(6)
O3 Cd2 O3 6 . 150.03(14)
O2 Cd2 O3 3_655 . 79.28(12)
O3 Cd2 O3 8_556 . 66.01(15)
O3 Cd2 Cl1 9 . 100.15(8)
O3 Cd2 Cl1 6 . 100.15(8)
O2 Cd2 Cl1 3_655 . 161.32(11)
O3 Cd2 Cl1 8_556 . 85.08(8)
O3 Cd2 Cl1 . . 85.08(8)
O3 Cd2 As1 9 . 116.95(8)
O3 Cd2 As1 6 . 116.95(8)
O2 Cd2 As1 3_655 . 73.07(11)
O3 Cd2 As1 8_556 . 33.23(7)
O3 Cd2 As1 . . 33.23(7)
Cl1 Cd2 As1 . . 88.254(19)
O3 Cd2 O1 9 4 61.91(9)
O3 Cd2 O1 6 4 61.91(9)
O2 Cd2 O1 3_655 4 99.31(13)
O3 Cd2 O1 8_556 4 146.83(8)
O3 Cd2 O1 . 4 146.83(8)
Cl1 Cd2 O1 . 4 99.37(8)
As1 Cd2 O1 . 4 172.38(8)
O3 Cd2 O1 9 3_655 67.08(9)
O3 Cd2 O1 6 3_655 67.08(9)
O2 Cd2 O1 3_655 3_655 51.18(13)
O3 Cd2 O1 8_556 3_655 121.37(10)
O3 Cd2 O1 . 3_655 121.37(10)
Cl1 Cd2 O1 . 3_655 147.50(7)
As1 Cd2 O1 . 3_655 124.25(7)
O1 Cd2 O1 4 3_655 48.13(14)
O3 Cd2 O3 9 4 55.29(8)
O3 Cd2 O3 6 4 92.21(8)
O2 Cd2 O3 3_655 4 136.97(11)
O3 Cd2 O3 8_556 4 143.65(9)
O3 Cd2 O3 . 4 115.32(12)
Cl1 Cd2 O3 . 4 59.71(5)
As1 Cd2 O3 . 4 140.81(5)
O1 Cd2 O3 4 4 45.72(8)
O1 Cd2 O3 3_655 4 90.02(8)
O3 Cd2 O3 9 11_556 92.21(8)
O3 Cd2 O3 6 11_556 55.29(8)
O2 Cd2 O3 3_655 11_556 136.97(11)
O3 Cd2 O3 8_556 11_556 115.32(12)
O3 Cd2 O3 . 11_556 143.65(9)
Cl1 Cd2 O3 . 11_556 59.71(5)
As1 Cd2 O3 . 11_556 140.81(5)
O1 Cd2 O3 4 11_556 45.72(8)
O1 Cd2 O3 3_655 11_556 90.02(8)
O3 Cd2 O3 4 11_556 40.58(10)
O1 As1 O3 . . 115.09(14)
O1 As1 O3 . 8_556 115.09(14)
O3 As1 O3 . 8_556 103.2(2)
O1 As1 O2 . . 111.0(2)
O3 As1 O2 . . 105.75(15)
O3 As1 O2 8_556 . 105.75(15)
O1 As1 Cd2 . . 141.11(17)
O3 As1 Cd2 . . 52.07(11)
O3 As1 Cd2 8_556 . 52.07(11)
O2 As1 Cd2 . . 107.90(16)
O1 As1 O2 . 3_655 175.25(19)
O3 As1 O2 . 3_655 67.36(12)
O3 As1 O2 8_556 3_655 67.36(12)
O2 As1 O2 . 3_655 64.3(2)
O1 As1 O3 . 10 57.47(14)
O3 As1 O3 . 10 60.75(13)
O3 As1 O3 8_556 10 110.90(15)
O2 As1 O3 . 10 142.92(9)
Cd2 As1 O3 . 10 90.66(6)
O2 As1 O3 3_655 10 126.13(8)
O1 As1 O3 . 5 57.47(14)
O3 As1 O3 . 5 110.90(15)
O3 As1 O3 8_556 5 60.75(13)
O2 As1 O3 . 5 142.92(9)
Cd2 As1 O3 . 5 90.66(6)
O2 As1 O3 3_655 5 126.13(8)
O3 As1 O3 10 5 65.26(10)
O1 As1 O2 . 7_666 64.73(7)
O3 As1 O2 . 7_666 159.26(14)
O3 As1 O2 8_556 7_666 61.85(13)
O2 As1 O2 . 7_666 92.78(10)
Cd2 As1 O2 . 7_666 113.73(7)
O2 As1 O2 3_655 7_666 114.59(6)
O3 As1 O2 10 7_666 109.07(9)
O3 As1 O2 5 7_666 50.14(9)
O1 As1 O2 . 7_665 64.73(7)
O3 As1 O2 . 7_665 61.85(13)
O3 As1 O2 8_556 7_665 159.26(14)
O2 As1 O2 . 7_665 92.78(10)
Cd2 As1 O2 . 7_665 113.73(7)
O2 As1 O2 3_655 7_665 114.59(6)
O3 As1 O2 10 7_665 50.14(9)
O3 As1 O2 5 7_665 109.07(9)
O2 As1 O2 7_666 7_665 127.63(13)
O1 As1 O3 . 2_665 63.89(15)
O3 As1 O3 . 2_665 157.52(13)
O3 As1 O3 8_556 2_665 96.67(11)
O2 As1 O3 . 2_665 58.07(13)
Cd2 As1 O3 . 2_665 143.54(5)
O2 As1 O3 3_655 2_665 112.19(8)
O3 As1 O3 10 2_665 121.19(9)
O3 As1 O3 5 2_665 87.84(10)
O2 As1 O3 7_665 2_665 101.09(8)
O1 As1 O3 . 7_665 63.89(15)
O3 As1 O3 . 7_665 96.67(11)
O3 As1 O3 8_556 7_665 157.52(13)
O2 As1 O3 . 7_665 58.07(13)
Cd2 As1 O3 . 7_665 143.54(5)
O2 As1 O3 3_655 7_665 112.19(8)
O3 As1 O3 10 7_665 87.84(10)
O3 As1 O3 5 7_665 121.19(9)
O2 As1 O3 7_666 7_665 101.09(8)
O3 As1 O3 2_665 7_665 62.03(10)
Cd2 Cl1 Cd2 4 . 120.0
Cd2 Cl1 Cd2 4 3 120.0
Cd2 Cl1 Cd2 . 3 120.0
Cd2 Cl1 O4 4 7_556 90.0
Cd2 Cl1 O4 . 7_556 90.0
Cd2 Cl1 O4 3 7_556 90.0
Cd2 Cl1 O4 4 7 90.0
Cd2 Cl1 O4 . 7 90.0
Cd2 Cl1 O4 3 7 90.0
O4 Cl1 O4 7_556 7 180.0
Cd2 Cl1 O3 4 8_556 150.42(5)
Cd2 Cl1 O3 . 8_556 46.28(5)
Cd2 Cl1 O3 3 8_556 79.71(5)
O4 Cl1 O3 7_556 8_556 66.73(5)
O4 Cl1 O3 7 8_556 113.27(5)
Cd2 Cl1 O3 4 3 79.71(5)
Cd2 Cl1 O3 . 3 150.42(5)
Cd2 Cl1 O3 3 3 46.28(5)
O4 Cl1 O3 7_556 3 113.27(5)
O4 Cl1 O3 7 3 66.73(5)
O3 Cl1 O3 8_556 3 125.31(2)
Cd2 Cl1 O3 4 4 46.28(5)
Cd2 Cl1 O3 . 4 79.71(5)
Cd2 Cl1 O3 3 4 150.42(5)
O4 Cl1 O3 7_556 4 113.27(5)
O4 Cl1 O3 7 4 66.73(5)
O3 Cl1 O3 8_556 4 125.31(2)
O3 Cl1 O3 3 4 105.41(6)
Cd2 Cl1 O3 4 12_556 79.71(5)
Cd2 Cl1 O3 . 12_556 150.42(5)
Cd2 Cl1 O3 3 12_556 46.28(5)
O4 Cl1 O3 7_556 12_556 66.73(5)
O4 Cl1 O3 7 12_556 113.27(5)
O3 Cl1 O3 8_556 12_556 105.41(6)
O3 Cl1 O3 3 12_556 46.55(11)
O3 Cl1 O3 4 12_556 125.31(2)
Cd2 Cl1 O3 4 . 150.42(5)
Cd2 Cl1 O3 . . 46.28(5)
Cd2 Cl1 O3 3 . 79.71(5)
O4 Cl1 O3 7_556 . 113.27(5)
O4 Cl1 O3 7 . 66.73(5)
O3 Cl1 O3 8_556 . 46.55(11)
O3 Cl1 O3 3 . 105.41(6)
O3 Cl1 O3 4 . 105.41(6)
O3 Cl1 O3 12_556 . 125.31(2)
Cd2 Cl1 O3 4 11_556 46.28(5)
Cd2 Cl1 O3 . 11_556 79.71(5)
Cd2 Cl1 O3 3 11_556 150.42(5)
O4 Cl1 O3 7_556 11_556 66.73(5)
O4 Cl1 O3 7 11_556 113.27(5)
O3 Cl1 O3 8_556 11_556 105.41(6)
O3 Cl1 O3 3 11_556 125.31(2)
O3 Cl1 O3 4 11_556 46.55(11)
O3 Cl1 O3 12_556 11_556 105.41(6)
O3 Cl1 O3 . 11_556 125.31(2)
Cd2 Cl1 O3 . 7 129.53(5)
Cd2 Cl1 O3 3 7 99.47(5)
O4 Cl1 O3 7_556 7 122.21(5)
O4 Cl1 O3 7 7 57.79(5)
O3 Cl1 O3 8_556 7 171.06(10)
O3 Cl1 O3 3 7 53.184(19)
O3 Cl1 O3 4 7 53.184(19)
O3 Cl1 O3 12_556 7 79.75(3)
O3 Cl1 O3 . 7 124.51(5)
O3 Cl1 O3 11_556 7 79.75(3)
Cd2 Cl1 H4 4 . 90.000(2)
Cd2 Cl1 H4 . . 90.0000(10)
Cd2 Cl1 H4 3 . 90.0000(10)
O4 Cl1 H4 7_556 . 180.000(3)
O3 Cl1 H4 8_556 . 113.27(6)
O3 Cl1 H4 3 . 66.73(5)
O3 Cl1 H4 4 . 66.73(5)
O3 Cl1 H4 12_556 . 113.27(5)
O3 Cl1 H4 . . 66.73(5)
O3 Cl1 H4 11_556 . 113.27(5)
O3 Cl1 H4 7 . 57.79(5)
As1 O1 Cd1 . 8_556 134.35(9)
As1 O1 Cd1 . . 134.35(9)
Cd1 O1 Cd1 8_556 . 89.36(15)
Cd1 O1 O2 8_556 . 119.83(15)
Cd1 O1 O2 . . 119.83(15)
Cd1 O1 O3 8_556 . 162.27(15)
Cd1 O1 O3 . . 107.06(8)
O2 O1 O3 . . 57.85(13)
Cd1 O1 O3 8_556 8_556 107.06(8)
Cd1 O1 O3 . 8_556 162.27(15)
O2 O1 O3 . 8_556 57.85(13)
O3 O1 O3 . 8_556 55.90(16)
As1 O1 O1 . 3_665 139.5(3)
Cd1 O1 O1 8_556 3_665 51.99(6)
Cd1 O1 O1 . 3_665 51.99(6)
O2 O1 O1 . 3_665 104.4(3)
O3 O1 O1 . 3_665 144.61(18)
O3 O1 O1 8_556 3_665 144.61(18)
As1 O1 O1 . 4_565 160.5(3)
Cd1 O1 O1 8_556 4_565 51.99(6)
Cd1 O1 O1 . 4_565 51.99(6)
O2 O1 O1 . 4_565 164.4(3)
O3 O1 O1 . 4_565 134.6(2)
O3 O1 O1 8_556 4_565 134.6(2)
O1 O1 O1 3_665 4_565 60.0
As1 O1 O3 . 10 95.19(17)
Cd1 O1 O3 8_556 10 118.95(19)
Cd1 O1 O3 . 10 65.69(10)
O2 O1 O3 . 10 120.94(14)
O3 O1 O3 . 10 64.53(12)
O3 O1 O3 8_556 10 99.61(18)
O1 O1 O3 3_665 10 115.38(14)
O1 O1 O3 4_565 10 70.09(18)
As1 O1 O3 . 5 95.19(17)
Cd1 O1 O3 8_556 5 65.69(10)
Cd1 O1 O3 . 5 118.95(19)
O2 O1 O3 . 5 120.94(14)
O3 O1 O3 . 5 99.61(18)
O3 O1 O3 8_556 5 64.53(12)
O1 O1 O3 3_665 5 115.38(14)
O1 O1 O3 4_565 5 70.09(18)
O3 O1 O3 10 5 79.12(17)
As1 O1 O2 . 7_666 88.14(11)
Cd1 O1 O2 8_556 7_666 46.31(8)
Cd1 O1 O2 . 7_666 134.75(17)
O2 O1 O2 . 7_666 84.40(11)
O3 O1 O2 . 7_666 118.11(16)
O3 O1 O2 8_556 7_666 62.70(11)
O1 O1 O2 3_665 7_666 86.81(12)
O1 O1 O2 4_565 7_666 94.12(11)
O3 O1 O2 10 7_666 136.82(17)
O3 O1 O2 5 7_666 57.71(10)
As1 O1 O2 . 7_665 88.14(11)
Cd1 O1 O2 8_556 7_665 134.75(17)
Cd1 O1 O2 . 7_665 46.31(8)
O2 O1 O2 . 7_665 84.40(11)
O3 O1 O2 . 7_665 62.70(11)
O3 O1 O2 8_556 7_665 118.11(16)
O1 O1 O2 3_665 7_665 86.81(12)
O1 O1 O2 4_565 7_665 94.12(11)
O3 O1 O2 10 7_665 57.71(10)
O3 O1 O2 5 7_665 136.82(17)
O2 O1 O2 7_666 7_665 165.3(2)
As1 O2 Cd2 . 4_665 121.0(2)
As1 O2 Cd1 . 7_665 107.50(16)
Cd2 O2 Cd1 4_665 7_665 114.10(14)
As1 O2 Cd1 . 2_665 107.50(16)
Cd2 O2 Cd1 4_665 2_665 114.10(14)
Cd1 O2 Cd1 7_665 2_665 87.53(15)
Cd2 O2 O3 4_665 . 135.24(16)
Cd1 O2 O3 7_665 . 70.97(11)
Cd1 O2 O3 2_665 . 110.49(18)
Cd2 O2 O3 4_665 8_556 135.24(16)
Cd1 O2 O3 7_665 8_556 110.49(18)
Cd1 O2 O3 2_665 8_556 70.97(11)
O3 O2 O3 . 8_556 58.51(17)
Cd2 O2 O1 4_665 . 87.05(17)
Cd1 O2 O1 7_665 . 128.02(12)
Cd1 O2 O1 2_665 . 128.02(12)
O3 O2 O1 . . 61.99(14)
O3 O2 O1 8_556 . 61.99(14)
As1 O2 O2 . 3_655 84.6(3)
Cd2 O2 O2 4_665 3_655 154.4(2)
Cd1 O2 O2 7_665 3_655 51.29(6)
Cd1 O2 O2 2_665 3_655 51.29(6)
O3 O2 O2 . 3_655 65.05(18)
O3 O2 O2 8_556 3_655 65.05(18)
O1 O2 O2 . 3_655 118.5(2)
As1 O2 O2 . 4_665 144.6(3)
Cd2 O2 O2 4_665 4_665 94.4(2)
Cd1 O2 O2 7_665 4_665 51.29(6)
Cd1 O2 O2 2_665 4_665 51.29(6)
O3 O2 O2 . 4_665 116.77(16)
O3 O2 O2 8_556 4_665 116.77(16)
O1 O2 O2 . 4_665 178.5(2)
O2 O2 O2 3_655 4_665 60.0
As1 O2 O3 . 11_666 151.47(12)
Cd2 O2 O3 4_665 11_666 51.19(10)
Cd1 O2 O3 7_665 11_666 99.70(16)
Cd1 O2 O3 2_665 11_666 64.59(10)
O3 O2 O3 . 11_666 170.03(19)
O3 O2 O3 8_556 11_666 124.24(14)
O1 O2 O3 . 11_666 127.98(17)
O2 O2 O3 3_655 11_666 106.59(15)
O2 O2 O3 4_665 11_666 53.26(15)
As1 O2 O3 . 4_665 151.47(12)
Cd2 O2 O3 4_665 4_665 51.19(10)
Cd1 O2 O3 7_665 4_665 64.59(10)
Cd1 O2 O3 2_665 4_665 99.70(16)
O3 O2 O3 . 4_665 124.24(14)
O3 O2 O3 8_556 4_665 170.03(19)
O1 O2 O3 . 4_665 127.98(17)
O2 O2 O3 3_655 4_665 106.59(15)
O2 O2 O3 4_665 4_665 53.26(15)
O3 O2 O3 11_666 4_665 51.18(14)
As1 O2 O3 . 2_665 95.04(16)
Cd1 O2 O3 7_665 2_665 155.74(18)
Cd1 O2 O3 2_665 2_665 94.30(8)
O3 O2 O3 . 2_665 129.90(16)
O3 O2 O3 8_556 2_665 92.88(12)
O1 O2 O3 . 2_665 68.36(13)
O2 O2 O3 3_655 2_665 142.77(7)
O2 O2 O3 4_665 2_665 112.76(18)
O3 O2 O3 11_666 2_665 60.02(11)
O3 O2 O3 4_665 2_665 91.31(15)
As1 O3 Cd2 . 10 132.49(17)
As1 O3 Cd2 . . 94.70(14)
Cd2 O3 Cd2 10 . 125.29(14)
Cd2 O3 O3 10 8_556 151.22(9)
Cd2 O3 O3 . 8_556 57.00(7)
Cd2 O3 O2 10 . 133.54(16)
Cd2 O3 O2 . . 100.20(13)
O3 O3 O2 8_556 . 60.74(9)
Cd2 O3 O1 10 . 100.94(13)
Cd2 O3 O1 . . 116.97(13)
O3 O3 O1 8_556 . 62.05(8)
O2 O3 O1 . . 60.16(15)
As1 O3 Cd1 . 7_665 86.44(13)
Cd2 O3 Cd1 10 7_665 111.40(13)
Cd2 O3 Cd1 . 7_665 94.77(10)
O3 O3 Cd1 8_556 7_665 96.23(6)
O2 O3 Cd1 . 7_665 49.32(10)
O1 O3 Cd1 . 7_665 106.37(14)
As1 O3 O1 . 9 131.42(18)
Cd2 O3 O1 10 9 78.21(11)
Cd2 O3 O1 . 9 90.27(12)
O3 O3 O1 8_556 9 129.56(8)
O2 O3 O1 . 9 94.18(15)
O1 O3 O1 . 9 144.23(17)
As1 O3 O2 . 3_655 82.08(13)
Cd2 O3 O2 10 3_655 142.16(14)
Cd2 O3 O2 . 3_655 49.53(10)
O3 O3 O2 8_556 3_655 64.41(7)
O2 O3 O2 . 3_655 61.69(19)
O1 O3 O2 . 3_655 114.11(14)
Cd1 O3 O2 7_665 3_655 46.43(9)
O1 O3 O2 9 3_655 65.16(9)
As1 O3 O3 . 9 137.2(2)
Cd2 O3 O3 10 9 89.29(13)
O3 O3 O3 8_556 9 101.30(12)
O2 O3 O3 . 9 123.26(16)
O1 O3 O3 . 9 160.14(18)
Cd1 O3 O3 7_665 9 85.18(11)
O1 O3 O3 9 9 54.34(13)
O2 O3 O3 3_655 9 62.22(12)
As1 O3 O3 . 10 91.25(17)
Cd2 O3 O3 10 10 50.47(10)
Cd2 O3 O3 . 10 116.73(10)
O3 O3 O3 8_556 10 101.30(12)
O2 O3 O3 . 10 119.88(16)
O1 O3 O3 . 10 61.13(14)
Cd1 O3 O3 7_665 10 148.49(14)
O1 O3 O3 9 10 128.68(18)
O2 O3 O3 3_655 10 163.60(17)
O3 O3 O3 9 10 116.25(8)
As1 O3 O2 . 7_665 90.48(13)
Cd2 O3 O2 10 7_665 47.72(9)
Cd2 O3 O2 . 7_665 172.60(15)
O3 O3 O2 8_556 7_665 127.22(8)
O2 O3 O2 . 7_665 87.12(12)
O1 O3 O2 . 7_665 65.77(9)
Cd1 O3 O2 7_665 7_665 90.82(12)
O1 O3 O2 9 7_665 90.26(13)
O2 O3 O2 3_655 7_665 136.78(15)
O3 O3 O2 9 7_665 131.44(17)
O3 O3 O2 10 7_665 57.76(13)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Cd1 O1 3_665 2.296(3)
Cd1 O1 4_565 2.296(3)
Cd1 O1 . 2.296(3)
Cd1 O2 10 2.375(3)
Cd1 O2 9_565 2.375(3)
Cd1 O2 7_665 2.375(3)
Cd1 O3 9_565 2.960(3)
Cd1 O3 10 2.960(3)
Cd1 O3 7_665 2.960(3)
Cd1 Cd1 8_556 3.2289(12)
Cd1 Cd1 8 3.2851(12)
Cd1 O3 4_565 4.125(3)
Cd2 O3 9 2.208(3)
Cd2 O3 6 2.208(3)
Cd2 O2 3_655 2.368(4)
Cd2 O3 8_556 2.426(3)
Cd2 O3 . 2.426(3)
Cd2 Cl1 . 2.5191(6)
Cd2 As1 . 3.0655(9)
Cd2 O1 4 3.372(5)
Cd2 O1 3_655 3.551(5)
Cd2 O3 4 3.811(3)
Cd2 O3 11_556 3.811(3)
As1 O1 . 1.656(4)
As1 O3 . 1.686(3)
As1 O3 8_556 1.686(3)
As1 O2 . 1.706(4)
As1 O2 3_655 3.283(4)
As1 O3 10 3.590(3)
As1 O3 5 3.590(3)
As1 O2 7_666 3.629(2)
As1 O2 7_665 3.629(2)
As1 O3 2_665 3.756(3)
As1 O3 7_665 3.756(3)
Cl1 Cd2 4 2.5191(6)
Cl1 Cd2 3 2.5191(6)
Cl1 O4 7_556 3.2570(5)
Cl1 O4 7 3.2570(5)
Cl1 O3 8_556 3.344(3)
Cl1 O3 3 3.344(3)
Cl1 O3 4 3.344(3)
Cl1 O3 12_556 3.344(3)
Cl1 O3 . 3.344(3)
Cl1 O3 11_556 3.344(3)
Cl1 O3 7 3.631(3)
Cl1 H4 . 0.89(2)
O1 Cd1 8_556 2.296(3)
O1 O2 . 2.770(6)
O1 O3 . 2.819(5)
O1 O3 8_556 2.819(5)
O1 O1 3_665 2.828(8)
O1 O1 4_565 2.828(8)
O1 O3 10 3.039(5)
O1 O3 5 3.039(5)
O1 O2 7_666 3.2839(10)
O1 O2 7_665 3.2839(10)
O2 Cd2 4_665 2.368(4)
O2 Cd1 7_665 2.375(3)
O2 Cd1 2_665 2.375(3)
O2 O3 . 2.704(5)
O2 O3 8_556 2.704(5)
O2 O2 3_655 2.970(8)
O2 O2 4_665 2.970(8)
O2 O3 11_666 3.059(5)
O2 O3 4_665 3.059(5)
O2 O3 2_665 3.200(5)
O3 Cd2 10 2.208(3)
O3 O3 8_556 2.643(7)
O3 Cd1 7_665 2.960(3)
O3 O1 9 3.039(5)
O3 O2 3_655 3.059(5)
O3 O3 9 3.133(7)
O3 O3 10 3.133(7)
O3 O2 7_665 3.200(5)
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0010346
